fatigue damage modeling in solder interconnects using a cohesive zone approach
International Journal of Solids and Structures 42 (2005) 927–942 www.elsevier.com/locate/ijsolstr Fatigue damage modeling in solder interconnects using a cohesive zone approach A. Abdul-Baqi, P.J.G. Schreurs *, M.G.D. Geers Department of Mechanical Engineering, Section of Materials Technology, Eindhoven University of Technology, P.O. Box 513, 5600 MB, Eindhoven, The Netherlands Received 19 May 2003; received in revised form 13 July 2004 Available online 12 October 2004Abstract The objective of this work is to model the fatigue damage process in a solder bump subjected to cyclic loading con-ditions. Fatigue damage is simulated using the cohesive zone methodology. Damage is assumed to occur at interfacesmodeled through cohesive zones in the material, while the bulk material is assumed to be linear elastic. The state ofdamage at a cohesive zone is incorporated into the cohesive zone constitutive law by a elasticity-based damage variable.The gradual degradation of the solder material and the corresponding damage accumulation throughout the cyclingprocess is accounted for by a damage evolution law which captures the main damage characteristics. The model pre-diction of the solder bump life-time is shown to be in good agreement with one of the commonly used empirical life-timeprediction laws.Ó 2004 Elsevier Ltd. All rights reserved.Keywords: Cohesive zone; Fatigue damage; Solder joint; Life-time1. Introduction In the electronics industry, reliability of an IC package is usually determined through the integrity of itssolder joint interconnects. The latter have the function of providing both electrical and mechanical connec-tions between the silicon chip and the printed circuit board. Repeated switching of the electronic deviceleads to temperature ﬂuctuations which, combined with the mismatch of the coeﬃcients of thermal expan-sion (CTE), will result in stresses causing fatigue of the solder joints. Progressive damage will eventually * Corresponding author. Tel.: +31 40 247 2778; fax: +31 40 244 7355. E-mail address: firstname.lastname@example.org (P.J.G. Schreurs).0020-7683/$ - see front matter Ó 2004 Elsevier Ltd. All rights reserved.doi:10.1016/j.ijsolstr.2004.07.026
928 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942result in a device failure. This problem is becoming increasingly important as the ﬂux of the dissipated en-ergy in the solder joints is increasing due to miniaturization. Numerical prediction of fatigue life-time of solder joints generally consists of four main steps. Firstly, aconstitutive model which describes the solder material behavior is chosen. Secondly, one loading cycle issimulated using the ﬁnite element method (FEM), where the stresses and the strains in the material are cal-culated. Thirdly, from the calculated stresses and/or strains, the number of cycles to failure Nf is calculatedbased on a selected fatigue life prediction model. A review of such models can be found in Lee et al. (2000).Finally, the model prediction is veriﬁed using experimental thermal cycling data. This approach is the mostpopular among other existing approaches for fatigue analysis of solder joints. This is mainly due to its sim-plicity and relatively short computing time. However, there is a major drawback associated with this ap-proach. The stresses and strains are calculated from a single loading cycle and the material properties ofthe solder are assumed to remain constant during the successive cycles. This assumption results in under-estimated values of the fatigue life because in reality, repeated cycling results in a gradual degradation of thesolder material (Basaran et al., 2001). This has been emphasized experimentally through the observationthat creep hysteresis loops of solder materials collapse over the thermal cycles (Zhang et al., 2000). More-over, solder joint fatigue models were developed based on experimental thermal cycling tests on macro-scopic specimens. The applicability of such models to a solder joint has not yet been justiﬁed. Morerealistic models should account for the microstructural evolution of the solder material during the processof cycling. During thermal and/or mechanical cyclic loading, the solder material undergoes phase separa-tion and severe coarsening at an early stage of the cycling process (Matin et al., 2003; Ubachs et al., 2003).The coarsening of the solder microstructure eventually leads to stress concentrations in the material which,in addition to the localization of the interfaces with the coarsened phases, will contribute severely to thefatigue damage. The incorporation of all such phenomena explicitly in a fatigue model is rather compli-cated. Instead, this can be achieved partially by adopting a continuum damage approach, for example,where the microstructural changes and the corresponding material degradation are accounted for in theconstitutive material model itself by a damage variable. However, besides the requirement of extensive com-putations, the choice of a damage variable and a damage evolution law is quite arbitrary and experimentalveriﬁcations are usually not available. The cohesive zone method is a numerical tool for the mechanics of interfaces, that was initially devel-oped to model crack initiation and growth. This method treats fracture as a gradual process in which sep-aration between incipient material surfaces is resisted by cohesive tractions (Nguyen et al., 2001). It is atypical interfacial damage model, which can be situated between continuum damage mechanics and frac-ture mechanics. In comparison with fracture mechanics, the cohesive zone method has the advantages ofsmoothing the stress singularities at the crack tip and the easy adaptability to material and geometrical non-linearities (Chaboche et al., 2001). Compared to continuum damage mechanics, the cohesive zone methodcan be used to model cracking at interfaces between dissimilar materials. The fracture characteristics of thematerial such as fracture energy (the area under the traction curve) and fracture strength (the peak cohesivetraction) are included in a typical cohesive zone constitutive relation. Consequently, crack initiation andcrack growth emerge as natural outcomes of the boundary value problem solution without any separatecriteria. In the past decade, the cohesive zone method was mainly applied to model cracking under mono-tonic loading conditions (Abdul-Baqi, 2002; Chaboche et al., 2001; Tijssens, 2000; Xu and Needleman,1993). The applicability of this method to fatigue damage under cyclic loading has only quite recentlystarted to receive some attention (de Andres et al., 1999; Nguyen et al., 2001; Roe and Siegmund, 2003;Yang et al., 2000). Damage, as a dissipative mechanism, can be accounted for explicitly by incorporatinga damage variable into the cohesive zone constitutive law (Roe and Siegmund, 2003). According to thisapproach the peak cohesive traction and cohesive energy are assumed to diminish with the damage param-eter. The damage is determined using an evolution law in which the damage rate is a function of the cohe-sive parameters. An other way to account for damage is to include an unloading–reloading hysteresis into
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 929the cohesive zone law (de Andres et al., 1999; Nguyen et al., 2001; Yang et al., 2000), that simulates theaccumulation of damage within the cohesive zone which eventually leads to complete failure. The objective of the present paper is to model the fatigue damage process in a solder bump subjected tocyclic loading. For this purpose we perform a numerical simulation of the load cycling process using theﬁnite element method. Damage in the bump is modeled using the cohesive zone methodology. Degradationof the solder material throughout the cycling process is accounted for by the incorporation of a damagevariable into the cohesive zone constitutive law. The damage variable is supplemented by an evolutionlaw to account for the accumulation of damage. The evolution law is typically phenomenological and isformulated in a way which takes into account the main damage characteristics. The cohesive zone descrip-tion proposed is applicable for quasi-brittle interfaces, i.e., where a degradation mechanism without notice-able permanent deformations is dominant. The presented model presents itself in a somewhat simplerformat than the Roe and Sigmund (Roe and Siegmund, 2003) approach, even though the damage evolutionlaw is more sophisticated. Damage evolution can be described for both normal and tangential directionsseparately. The evolution law contains more parameters, which can be used to describe the damage evolu-tion more accurately, especially at the ﬁnal stage of the life-time. Damage distribution in the solder bump ispresented at diﬀerent loading cycles and at complete failure. The decrease of the reaction force with thenumber of cycles is illustrated as a measure of the overall loss of stiﬀness. Finally, the life-time predictioncapability of the model is compared with the prediction of one of the commonly used classical models, aCoﬃn–Manson law. So far, the analysis is limited to a two-dimensional conﬁguration, where the thirddimension is constrained through a plane strain assumption.2. Problem formulation Solder materials undergo continuous microstructural coarsening during loading. Fig. 1 illustrates suchcoarsened microstructure for a eutectic tin–lead (Sn–Pb) solder after only 48 h of thermal ageing. Fornumerical convenience, the present simulations are performed on a rather simpliﬁed microstructure as illus-trated in Fig. 2. A single solder bump is modeled in plane-strain which is an approximation of the actualthree-dimensional problem. The solder material which is assumed to be a eutectic tin–lead solder is Fig. 1. Tin–lead solder with the white region being the lead-rich phase (Matin et al., 2003).
930 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 Fig. 2. Modeled geometry.idealized as a well-deﬁned two-phase system. The inclusions are assumed to be the lead-rich phase, while thesurrounding bulk is the tin-rich phase. Fatigue damage in the bump is modeled using a cohesive zone ap-proach as explained in Section 2.1. Cohesive zones are embedded at physical boundaries in the solder bump(interfaces with the upper and lower boundaries and interfaces with the second phase inclusions) as well asat the grain boundaries of the same phase. Experimentally, it has been observed that fatigue damage indeedlocalizes at these physical interfaces, which motivates the use of the cohesive zone approach adopted here.Cyclic loading is applied in terms of sinusoidal shear displacement which is prescribed incrementally alongthe upper boundary while keeping the lower boundary ﬁxed. The bump material is assumed to be linear elastic with a YoungÕs modulus E = 50 GPa and a PoissonÕsratio m = 0.36 for the bulk (tin phase) and E = 16 GPa and m = 0.44 for the inclusions (lead phase). Theupper and lower layers are assigned the same values as those of tin. Evidently, the full characterizationof solder joint fatigue would necessitate the incorporation of cyclic thermal loading and temperature relatedmaterial modeling (creep) and consequently the quantiﬁcation of temperature dependent material param-eters. Temperature and rate dependence are not yet incorporated in this framework. Even though the bulkphases indeed show a typically viscoplastic response, failure is experimentally found to localize at physicalinterfaces (interphase boundaries, colony boundaries, etc.), where the proposed model serves as a good ﬁrstapproximate. The sinusoidal shear displacement has an amplitude of 1.0 lm which results in a maximum applied shearstrain max = 1.0%. The analysis is carried out numerically using the ﬁnite element method. It uses a totalLagrangian formulation in which equilibrium is expressed in terms of the principle of the virtual work as Z Z Z rij dij dv þ T a dDa dS ¼ ti dui ds ð1Þ v Si @vHere, v is the total region analyzed and ov is its external boundary. With xi = (x, y, z) the coordinates, ui andti are the components of displacement and traction vector, respectively; rij are the components of Cauchystress while ij are the linear strain components. The latter are expressed in terms of the displacement ﬁeldsin the standard manner, 1 oui ouj ij ¼ þ ð2Þ 2 oxj oxi
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 931 The second term in the left-hand side of Eq. (1) is the contribution of the cohesive zones. The tractiontransmitted across a cohesive zone has components Ta, while the opening displacement is Da, both meas-ured in a local frame of reference at the cohesive zone. The cohesive zone nodal force vector and stiﬀnessmatrix are derived in Section 2.2. The previous equations, completed with the constitutive law for the cohesive zones to be discussedfurther on, form a nonlinear problem that is solved incrementally using the rate form of the virtual workin Eq. (1). The numerical procedure used to solve the present boundary value problem follows the one usedby Wu and van der Giessen (1996).2.1. Cohesive tractions and damage evolution A cohesive zone is a four-noded element (Fig. 3) with zero initial thickness (D = 0). Its constitutivebehavior is speciﬁed through a relation between the relative opening displacement Da and a correspondingtraction Ta at the same location, with a being either the local normal (n) or tangential (t) direction in thecohesive zone plane (Abdul-Baqi, 2002). For the case of monotonic loading, the cohesive traction is char-acterized mainly by a peak value which represents the cohesive strength and a cohesive energy. An exampleof such tractions are those given by Xu and Needleman (1993): Dn Dn T n ¼ rmax expð1Þ exp À ð3Þ dn dn ! pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Dt D2t T t ¼ smax 2 expð1Þ exp À 2 ð4Þ dt dtwhere dn and dt are characteristic lengths, rmax and smax are the peak tractions in the normal and tangentialdirections, respectively. Energy dissipation is accounted for by the softening branch in the curve as illus-trated in Fig. 4. Under monotonic loading, the cohesive traction reaches a peak value when a critical open-ing displacement is attained then starts to diminish with the gradual increase of the opening displacement.This will result in the creation of two traction-free surfaces which marks the initiation of a crack or theextension of an existing one. Under cyclic loading, the situation is rather diﬀerent. If the applied traction is less than the cohesivestrength, the cohesive zone will have an inﬁnite life. Fatigue experiments, however, indicate that under cyc-lic loading materials fail at stress levels below their static fracture strength (Ellyin, 1997) which is essentially continuum element 3 n 4 cohesive zone midplane t ∆ 1 2 continuum elementFig. 3. Cohesive zone illustration. (t, n) is a local frame of reference deﬁned such that the t-axis lies in the cohesive zone midplane.
932 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 1 1 max t max 0 T /σ T /τ n 0 –1 (a) –1 (b) –2 1 0 1 2 3 4 5 6 –3 –2 –1 0 1 2 3 ∆n/δn ∆t/δt Fig. 4. Cohesive zone monotonic normal (a) and shear (b) tractions.due to creep damage. Following the formulation of Chaboche et al. (2001), in the present study we adopt aconstitutive law in which the traction is a linear function of the separation, whereas the energy dissipation isaccounted for by the incorporation of a nonlinear damage variable into the constitutive law: T a ¼ k a ð1 À Da ÞDa ð5Þwhere ka is the initial stiﬀness of the cohesive zone and Da is the damage variable. Da varies between zero (0)for damage-free cohesive zones and one (1) for completely damaged zones. In this formulation, energy dis-sipation associated with the gradual degradation of the solder material is accounted for by the damage var-iable Da only. An additional softening branch emerging from a nonlinear traction law would add anadditional energy dissipation mechanism. The damage variable is supplemented with an evolution law to account for the accumulation of damagethroughout the cycling process. Motivated by the formulation of Roe and Siegmund (2003), the followingevolution law is here adopted: D_ a ¼ ca j Da j ð1 À Da þ rÞm j T a j À rf _ ð6Þ 1 À Da _where ca is a constant which controls the damage accumulation, Da is the rate of the relative opening of thecohesive zone, r and m are constants which control the decay of the reaction force at the ﬁnal stage of dam-age and rf is the cohesive zone endurance limit (Roe and Siegmund, 2003). Note that static strength of thecohesive zone, i.e., the maximum load after which abrupt softening would occur, is never reached in thismodel. In practice, this assumption is based on the fact that the bulk material of interest will yield and de-form plastically before this maximum load is reached. Note that monotonous damage relies on diﬀerentdissipation mechanisms, which can be added to the model in a similar manner as Roe and Sigmund did.Since these mechanisms are not considered here, monotonous damage has been ignored. In the next section,the main features of the damage evolution law (Eq. (6)) together with the traction separation law (Eq. (5))are examined against the main cyclic damage characteristics.2.2. Cohesive zone virtual work The contribution of the cohesive zones to the virtual work principle in Eq. (1) is determined by calcu-lating the cohesive zone stiﬀness matrix and internal nodal force vector. In the local frame of reference(t, n) illustrated in Fig. 3, the cohesive element nodal displacement vector is given by
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 933 uT ¼ fu1 ; u1 ; u2 ; u2 ; u3 ; u3 ; u4 ; u4 g l t n t n t n t n ð7Þwhere subscript l denote quantities in the local frame of reference. The local relative displacement vector Dis given as Dt D¼ ¼ Aul ð8Þ Dnwhere A is a matrix of the shape functions given as # Àh1 0 Àh2 0 h1 0 h2 0 A¼ ð9Þ 0 Àh1 0 Àh2 0 h1 0 h2and 1 1 h1 ¼ ð1 À gÞ; h2 ¼ ð1 þ gÞ ð10Þ 2 2The parameter g is deﬁned at the cohesive zone mid plane and varies between À1 at nodes (1, 3) and 1 atnodes (2, 4). The element internal nodal force vector and stiﬀness matrix are now written as Z Z þ1 l fl ¼ AT T dS ¼ AT T dg ð11Þ S 2 À1 Z Z þ1 l Kl ¼ AT DA dS ¼ AT DA dg ð12Þ S 2 À1where T is the traction vector corresponding to the displacement D and calculated via Eq. (5), S is the cohe-sive zone area and l is the cohesive zone length. This formulation is for plane-strain conditions and thecohesive zones are assumed to have a unit thickness. D is the cohesive zone constitutive tangent operatorthat relates the incremental variations of the tractions, dT, to the incremental variations of the displace-ments, dD, within the cohesive zone as dT ¼ D dD; ð13Þwhere 2 3 oT t oT t 6 oDt oDn 7 6 7 D¼6 7: ð14Þ 4 oT n oT n 5 oDt oDnThe integrals in Eqs. (11) and (12) are evaluated using Gaussian integration. Once the element internal no-dal force vector fl and stiﬀness matrix Kl are constructed in the local frame of reference (t, n), they are trans-formed to the global frame of reference (x, y, z) as f ¼ RT f l ð15Þ K ¼ RT Kl R ð16Þ
934 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 2 3 R0 0 0 0 60 R0 0 0 7 6 7 R¼6 7 ð17Þ 40 0 R0 0 5 0 0 0 R0where R 0 is the rotation matrix which relates the local frame to the global frame and is given in terms of theangle h between the t- and x-axes 0 cos h sin h R ¼ ð18Þ À sin h cos h3. Results and discussion3.1. Uniaxial cyclic tension–compression In this section, the fatigue damage constitutive model is demonstrated in a one-dimensional case as illus-trated in Fig. 5. The bar has a length L = 2 · 10À2 mm and a radius R = 10À2 mm. It is assumed to be linearelastic with E = 30 GPa and m = 0.25. Loading is applied in terms of a sinusoidal axial displacement U withan amplitude Uo = 2 · 10À4 mm. A single cohesive zone with an initial stiﬀness k = 106 GPa/mm is placed inthe middle of the bar to account for fatigue damage. The value taken for the initial stiﬀness will be com-mented on later in this section. For the damage evolution law (Eq. (6)) we have used c = 100 mm/N,rf = 150 MPa, r = 10À3 and m = 3. In this section, subscripts are irrelevant and hence omitted. The initial stiﬀness of the cohesive zones has to be suﬃciently high in order to diminish their artiﬁcialenhancement of the overall compliance (Tijssens, 2000; Xu and Needleman, 1993). In this one-dimensionalmodel, this enhancement can be analytically assessed from the stress continuity requirement. If we assume Fig. 5. Uniaxial tension–compression bar.
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 935that the bar contains n equally spaced cohesive zones, each having the same opening D, the stress r in thecontinuum and the traction T at the cohesive zone are given by: ðU À nDÞ r¼ E ð19Þ L T ¼ kð1 À DÞD ð20ÞAfter the opening D is obtained from the continuity requirement, r = T, and substituted in Eq. (19), we getan expression for the stress, r = (U/L)E*, where E* is an apparent elastic modulus given as ! 1 EÃ ¼ 1 À kL E ð21Þ nE ð1 À DÞ þ 1To ensure a negligible enhancement of the overall compliance, it is essential that the condition nE ( 1 is kLsatisﬁed. For the parameters used in this section, nE ¼ 1:5 Â 10À3 , which is suﬃciently small. In a two- kL Edimensional model the condition is estimated by kl ( 1, where l % L/n is the average cohesive zone length. The evolution of damage with the number of load cycles is shown in Fig. 6(a). In agreement with exper-imental observations (Kanchanomai et al., 2002), the presence of a mean strain is seen to cause more dam-age. Eq. (6) results in a nonlinear damage accumulation as illustrated in Fig. 6(b). In the high–low (H–L)sequence, 200 cycles are applied at a strain of 1% then followed by 200 cycles at 0.5% strain. The order isreversed for the (L–H) sequence. The model prediction is in agreement with experimental observationswhich indicate that cycling at a high stress level followed by cycling at a lower level (H–L) causes moredamage than when the order is reversed (L–H) (Fatemi and Yang, 1998). This is explained by the fact thatmicrocracks are generated during the ﬁrst loading block and grow during the second block. Starting withthe high loading block will cause more microcracks which will eventually grow during the second blockcausing more damage in the material. Assuming a zero value of the endurance limit rf in Eq. (6), both loadsequences would result in the same amount of damage. In this case, damage accumulation would be linearas assumed in the classical MinerÕs law. It is stated in Lemaitre (1996) that all damage laws of the followinggeneral shape show a property of linear accumulation: _ D ¼ f1 ðDÞf2 ðxÞ_ x ð22Þwhere x can either be a stress or a strain. For rf = 0, Eq. (6) can be rewritten in the form of Eq. (22). 1 1 HL 0.8 0.8 LH ε =0 mean 0.6 εmean = 0.5 % 0.6 D D 0.4 0.4 0.2 0.2 (a) (b) 0 0 0 200 400 600 800 1000 0 100 200 300 400 N (cycles) N (cycles) Fig. 6. Damage evolution with loading cycles. (a) Mean strain eﬀect and (b) load sequencing eﬀect.
936 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 400 0.15 (a) 0.1 (b) 200 0.05 T (MPa) F (N) 0 0 –0.05 –200 –0.1 –400 –0.15 –0.05 0 0.05 0.1 0.15 0.2 0 200 400 600 800 1000 ∆ (µm) N (cycles) Fig. 7. (a) Cohesive traction versus opening and (b) reaction force versus the number of cycles. The cohesive traction is shown in Fig. 7(a) as a function of the opening displacement D. As damage in-creases gradually to one, the stiﬀness and traction diminish to zero. Under compression, the cohesive zoneis assumed to maintain its initial stiﬀness as also seen in Fig. 7(a). This is achieved by using a zero value forthe damage variable in Eq. (6) whenever the relative opening displacement D is negative. The physical inter-pretation of this assumption is that the cohesive zone does not soften under compression. Numerically, itminimizes the interpenetration of neighboring continuum elements when they are in a compression state.This assumption is based on the monotonic normal traction shown in Fig. 4(a), in which the stiﬀness inthe negative D region is maintained high. The maximum traction in Fig. 7(a) is seen to decrease linearlywith the maximum opening displacement. This relation is also reﬂected in Eq. (19). The decrease of thereaction force is shown in Fig. 7(b). The ﬁgure shows a slow decrease at the initial loading stage followedby rapid decrease. This behavior is governed by both the constants m and r in the evolution law. Lowervalue of the exponent m leads to a brittle-like behavior in which the force will suddenly drop to zero. Thisis illustrated in Fig. 8(a) for m = 1. For r = 0, the behavior is illustrated in Fig. 8(b). The rapid decreasestage of the reaction force is followed by a stage of very slow decrease. 0.15 0.15 0.1 (a) 0.1 (b) 0.05 0.05 F (N) F (N) 0 0 –0.05 –0.05 –0.1 –0.1 –0.15 –0.15 0 20 40 60 80 100 0 500 1000 1500 2000 N (cycles) N (cycles)Fig. 8. Reaction force versus the number of cycles for two combinations of the constants r and m in the damage law. (a) r = 10À3,m = 1 and (b) r = 0, m = 3.
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 9373.2. Damage in a solder bump The bump model (Fig. 2) is analyzed using quadrilateral four-node elements. Cohesive zones are placedalong physical interfaces, i.e., grain boundaries, phase boundaries and colony boundaries. Consequently,each element represents a physical domain which is characteristic for the underlying microstructure. Theﬁnite element discretization is therefore inherently coupled to the microstructure. Cohesive zones in the solder bump are assigned the same value for the initial stiﬀness ka = 106 GPa/mm.This stiﬀness is suﬃciently high compared to the continuum stiﬀness such that, in the absence of damage,the cohesive zones artiﬁcial enhancement of the overall compliance is negligible. For the current geometry(Fig. 2), this has been veriﬁed through the observation that using higher values for the initial stiﬀness haslead to identical reaction forces at the ﬁrst cycle. The distinction between the diﬀerent cohesive zone groups is made by assigning diﬀerent values for thecoeﬃcient ca in the evolution law. For those at the interfaces with the upper and lower boundaries (i.e. atthe Copper pads), czg1 in Fig. 2, ca = 0. This is to prevent the early failure at these locations which is notobserved in practice, which would diminish the load transmitted to the bump and hence would stop thepropagation of damage into the bump. Inside the bump, cohesive zones at the interface with the secondphase inclusions (i.e. the interphase boundary), czg3, are assigned the highest value ca = 100 mm/N. Thisis based on experimental observations in which fatigue damage is found to occur mainly along these inter-faces. Inside the inclusions (i.e. the grain boundaries of the lead-rich phase), czg3, ca = 0. For the group czg2(i.e. the grain boundaries of the tin-rich phase), ca = 25 mm/N. The remaining parameters are rf = 0,r = 10À3 and m = 3. For each group the above parameters assume the same value in the tangential(a = t) and in the normal (a = n) directions. The detailed simulation of an individual cycle is time consuming, especially for a large number of cycles.In order to reduce the computational time, a method is adopted where only selected cycles are simulatedand the contribution of others is extrapolated. Damage is the only history dependent variable in the sim-ulation and hence it is the only extrapolated one. After a detailed simulation of a speciﬁc number of cycles,the damage variable Da(N) is ﬁtted with the cycle number by a third-degree polynomial using the data of theprevious 10 cycles. Now the cycle number is increased by an increment DN and the damage variable at thecurrent cycle is extrapolated as Da(N + DN). The increment of cycles is chosen so that the damage incrementDa(N + DN) À Da(N) is suﬃciently small (de Andres et al., 1999). The distribution of damage at diﬀerent cycles is shown in Fig. 9. At each cohesive zone an eﬀective dam-age value is calculated from the normal and tangential damage components at that location as 2 2 1=2 Dieff ¼ ðDit þ Din À Dit Din Þ : ð23ÞA cohesive zone (i) is marked as damaged when Dieff P 0:5. Fig. 9 shows that damage initiates close to theupper and lower boundaries and at the center of the bump. Later on, damage propagates to the interfaceswith the second phase inclusions, then throughout the entire bump leading to complete failure. As damage progresses in the solder bump, the overall stiﬀness decreases and the load required to attainthe same strain level decreases as shown in Fig. 10. The ﬁgure shows a slow softening at the initial stagefollowed by rapid softening. This qualitative behavior is in agreement with experimental observations ontin–lead solder alloys (Kanchanomai et al., 2002). An eﬀective measure of the total damage in the solder bump is computed by averaging the eﬀective dam-age given by Eq. (23) over the entire bump, i.e., 1X i i N cz Deff ¼ D A ð24Þ A i¼1 eff
938 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 Fig. 9. Damage distribution in the solder bump at diﬀerent cycles. White lines indicate damaged cohesive zones. 8 6 4 2 F (N) 0 x –2 –4 –6 –8 0 2000 4000 6000 8000 N (cycles) Fig. 10. The reaction force versus the number of cycles.where Ai is the ith cohesive zone area, A is the total area and Ncz is the number of cohesive zones. The evo-lution of the total eﬀective damage throughout the cycling process is shown in Fig. 11. The ﬁgure shows arapid increase of damage at the initial cycling stage and a much slower increase at the ﬁnal stage. This canbe explained by the fact that initially more cohesive zones are damaged as the load is transmitted throughthe entire bump. At a later stage all cohesive zones close to the boundaries are damaged as seen in the
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 939 0.5 0.4 0.3 Deff 0.2 0.1 0 0 2000 4000 6000 8000 N (cycles) Fig. 11. The total eﬀective damage versus the number of cycles.Figure after 2000 cycles. The load transmitted through these damaged bands starts to decrease rapidly. As aconsequence, the deformation of the cohesive zones in between decreases as well as their contribution to thetotal damage. The latter is a typical illustration of the localization that develops progressively in fatigue. To establish the number of cycles to failure and the associated fatigue life-time, an appropriate fatiguefailure criterion has to be chosen. As the simulation is performed under strain-controlled conditions, thedecrease of the reaction force has been chosen as a failure indicator. Failure of the bump is assumed tooccur when the reaction force reaches a critical value. This value is taken as 50% of the maximum forceat the ﬁrst cycle (Kanchanomai et al., 2002; Lee et al., 2000). For an applied strain max ranging from0.2% to 10% the corresponding number of cycles to failure Nf is calculated. The results presented in Fig.12 follow a typical (S–N) type of behavior and they are well-ﬁtted with a Coﬃn–Manson model, b max ¼ að2N f Þ ð25Þwhere a is the fatigue ductility coeﬃcient and b is the fatigue ductility exponent. In here, max is themaximum overall strain, which is deﬁned as the maximum applied displacement divided by the solderbumpÕs width. The sensitivity of the parameters a and b with respect to the chosen failure criterion is also 0.5 FEM linear fit 1 1.5 log(εmax) 2 2.5 3 1 2 3 4 5 6 log(2Nf)Fig. 12. The applied strain max versus the number of reversals to failure 2Nf. Discrete points are numerical results, solid line is a linearﬁt with max = 0.83(2Nf)À0.49.
940 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 4 3 f r N /N 2 f 1 0 0.5 0.75 1 1.25 1.5 E/E rFig. 13. Variation of the number of cycles to failure with the YoungÕs moduli at constant maximum strain max = 1%. N r ¼ 3899 is the fnumber of cycles to failure for the reference case with Er = 50 and 16 GPa for the tin-rich and lead-rich phases, respectively. E is amultiple of these values. Discrete points are numerical results, solid line is a ﬁt with: N f =N r ¼ ðE=Er ÞÀ1:83 . finvestigated. Using critical values of 25% and 75% resulted in the same value for the exponent b, namely,À0.49. The coeﬃcient a is found to depend on the failure criterion. Values of 1.0 and 0.69 are obtainedusing the 25% and the 75% criterion, respectively. The value obtained for the exponent b is within the rangeof experimentally obtained values for solder alloys (Kanchanomai et al., 2002; Lee et al., 2000). The sensitivity of the parameters a and b in Eq. (25) to the elastic properties of the solder bump is alsoinvestigated. Two sets of calculations were performed using YoungÕs moduli which are 50% lower and 50%higher than those listed in Section 2. The results of both sets were also well-ﬁtted with a Coﬃn–Mansonmodel. The values of the exponent b obtained for both sets are less than 1% diﬀerent from 0.49 which isobtained previously for the data listed in Section 2. The coeﬃcient a, however, is found to be dependenton the elastic moduli. Compared to the previous value of 0.83, values of 0.59 and 1.6 are obtained forthe higher and lower YoungÕs moduli, respectively. This leads to the conclusion that the higher the YoungÕsmoduli, the smaller the number of cycles to failure. Fig. 13 shows the number of cycles to failure as a func-tion of the changes in the YoungÕs moduli of the bump. It is clear from the ﬁtting exponents in Figs. 12 and13 that the dependence of the number of cycles to failure on the elastic moduli is as strong as their depend-ence on the applied strain. For the range of applied strains 0.2–10%, the reaction force and the total eﬀective damage show somescaling behavior. The reaction force normalized by the corresponding maximum force at the ﬁrst cycleF x ðN Þ=F max versus the normalized number of cycles N/Nf is identical for all values of applied strain. The xsame holds for the total eﬀective damage Deﬀ when plotted against N/Nf. The shape of these plots lookslike the shape like their respective ones in Figs. 10 and 11. This scaling holds only when rf = 0 in the dam-age evolution law of Eq. (6), which is the case here. In fact, this simply illustrates that damage accumulationis linear in this case. From the one-dimensional model discussed in Section 3.1 it is found that this scalingdoes not hold anymore for a nonzero value of the endurance limit as a result of a nonlinear damageaccumulation.4. Concluding remarks Fatigue damage in a solder bump has been simulated in this paper using the ﬁnite element method.Damage is modeled using the cohesive zone method in which cohesive zones are embedded at physical
A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942 941boundaries or interfaces which are potential locations for failure. The constitutive behavior of the cohesivezone is speciﬁed by a linear relation between the relative opening displacement at the cohesive zone and acorresponding traction. Material nonlinearity associated with dissipative mechanisms is accounted for bythe inclusion of a damage variable into the cohesive zone constitutive law. The damage variable is supple-mented with an evolution law to account for the gradual degradation of the solder material and the corre-sponding accumulation of damage throughout the cycling process. The evolution law is formulated suchthat it captures the main experimentally observed fatigue damage characteristics. The cohesive zone approach seems promising in modeling fatigue damage in solder alloys. The numer-ical model prediction of the solder bump life-time was shown to have a good agreement with the Coﬃn–Manson model which has been one of the most common engineering models used for fatigue life-timepredictions. The value obtained for the fatigue ductility exponent lies within the range of experimentallyobtained values for solder alloys. It was demonstrated that this value does not depend on the variationsin the elastic properties of the solder bump nor on the chosen failure criteria. The predicted life-time, how-ever, was found to have a dependence on the elastic moduli of the bump as strong as its dependence on theapplied strain. The detailed simulation of each individual cycle is yet time consuming, especially for more realisticmicrostructure and large number of cycles. The time-reduction method explained in this study is only partlyeﬃcient since it still requires a detailed simulation of a large number of cycles. A major gain in the com-putational time can be achieved by the use of a time homogenization technique, which constitutes futurework. In conclusion, the original aspects of this work can be summarized as: (1) elaboration of a cohesive zoneconstitutive model for macroscopically quasi-brittle interfaces, using an elasticity-based damage formula-tion with a complex yet ﬂexible description of the damage evolution; (2) elaboration of a constitutive modelthat enables the use of a relatively high initial stiﬀness, which avoids debatable assumptions that aﬀect theoverall compliance and which is a requirement for materials that fail in a quasi-brittle manner at the level ofan interface; (3) application to a particular material of interest, solders in micro-electronics joints, for whichit is known that failure concentrates at interfaces. This example illustrates that a ÔsimpleÕ elasticity-baseddamage interfacial model already predicts the main trends observed (particularly in comparison with empir-ical fatigue models), in spite of the fact that the bulk material is not yet characterized nonlinearly, i.e., as aviscoplastic material.Acknowledgment This research is a part of the BTS-Senter project RIPOSTE (no. BTS99133), in cooperation with PhilipsCenter for Industrial Technology and Philips Research Laboratory Eindhoven.ReferencesAbdul-Baqi, A., 2002. Failure of Brittle Coatings on Ductile Metallic Substrates. PhD thesis, Shaker Publishing, The Netherlands.Basaran, C., Tang, H., Dishong, T., Searls, D., 2001. Computer simulations of solder joint reliability tests. Advanced Packaging.Chaboche, J., Feyela, F., Monerie, Y., 2001. Interface debonding models: a viscous regularization with a limited rate dependency. International Journal of Solids and Structures 38, 3127–3160.de Andres, A., Perez, J., Ortiz, M., 1999. Elastoplastic ﬁnite element analysis of three-dimensional fatigue crack growth in aluminum shafts subjected to axial loading. International Journal of Solids and Structures 36, 2231–2258.Ellyin, F., 1997. Fatigue Damage, Crack Growth and Life Prediction. Chapman Hall.Fatemi, A., Yang, L., 1998. Cumulative fatigue damage and life prediction theories: a survey of the state of the art for homogeneous materials. International Journal of Fatigue 20, 9–34.
942 A. Abdul-Baqi et al. / International Journal of Solids and Structures 42 (2005) 927–942Kanchanomai, C., Miyashita, Y., Mutoh, Y., 2002. Low cycle fatigue behavior and mechanisms of a eutectic Sn–Pb solder 63Sn/37Pb. International Journal of Fatigue 24, 671–683.Lee, W., Nguyen, L., Selvaduray, G., 2000. Solder joint fatigue models: review and applicability to chip scale packages. Microelectronics Reliability 40, 231–244.Lemaitre, J., 1996. A Course on Damage Mechanics. Springer-Verlag, Berlin.Matin, M., Vellinga, W., Geers, M., 2003. Quantitative microscopy of microstructural evolution in eutectic solders subjected to static thermal load. In: Proceedings of the EuroSimE 2003 Conference, Aix-en-Provence, France.Nguyen, O., Repetto, E., Ortiz, M., Radovitzky, R., 2001. A cohesive model of fatigue crack growth. International Journal of Fracture 110, 351–369.Roe, K., Siegmund, T., 2003. An irreversible cohesive zone model for interface fatigue crack growth simulation. Engineering Fracture Mechanics 70, 209–232.Tijssens, M., 2000. On the cohesive surface methodology for fracture of brittle heterogeneous materials. PhD thesis, Shaker Publishing, The Netherlands.Ubachs, R., Schreurs, P., Geers, M., 2003. Microstructure evolution of tin–lead solder. In: Proceedings of the EuroSimE 2003 Conference, Aix-en-Provence, France.Wu, P., van der Giessen, E., 1996. Computational aspects of localized deformations in amorphous glassy polymers. European Journal of Mechanics, A/Solids 15, 799–823.Xu, X.-P., Needleman, A., 1993. Void nucleation by inclusion debonding in a crystal matrix. Modelling and Simulation in Materials Science and Engineering 1, 111–132.Yang, B., Mall, S., Ravi-Chandar, K., 2000. A cohesive zone model for fatigue crack growth in quasibrittle materials. International Journal of Solids and Structures 38, 3927–3944.Zhang, X., Lee, S.-W., Pao, Y.-H., 2000. A damage evolution model for thermal fatigue analysis of solder joints. Journal of Electronic Packaging 122, 200–206.